C 6 Planning resources for 84, Annex Coating materials for wear-resistant coatings: thin coatings General description of material: two-component coating material subst. No 684.30: PUR-hot sprayed material subst. No 684.31: PUR-smoothing cement for repairing the PUR-hot sprayed material subst. No 684.32: EP/PUR-smoothing cement, workable with airless application subst. No 684.33: PUR-sprayed material, workable with airless application or manually Additional notes: object temperature at least 5 °C and at least 3 K above dew point) Table C 4.3.6: Planning resources for materials according to Sheet 84, Annex Area of application Protective system Application Minimum waiting time before System structure Surface Nominal dry film subsequent preparation thicknesses [μm] coating at approx. 20 °C dry wet Vertical and inclined No 684.30/33 ,) Sa 2½ 2000 2000 hot spraying; , ) surfaces of workable manually or by - roadway slabs that airless are in contact with application ballast - riveted and welded spray subst. No 2000 2000 process deck bridges und 684.322), then manually or by trough bridges intersperse quartz airless sand 0.4 - 0.7 mm application subst. No 684.51 horizontal surfaces of subst. No 684.30/33 Sa 2½ 4000 4000 hot spraying; 4, 5) 2,3) workable - roadway slabs that manually or by are in contact with airless ballast application - riveted and welded deck bridges and subst. No 4000 4000 process trough bridges 684.322), then manually or by intersperse quartz airless sand 0.4 - 0.7 mm application subst. No 684.51 tread-resistant walkway No 684.32/332) Sa 2½ 2000 2000 as above 4) surfaces under heavy then intersperse quartz traffic sand 0.4 - 0.7 mm subst. No 684.51 substances as per Sheet 84, Annex are not suitable: as GB for other TL substances. −
C 6 Planning resources for 84, Annex Coating materials for wear-resistant coatings: thin coatings General description of material: two-component coating material subst. No 684.30: PUR-hot sprayed material subst. No 684.31: PUR-smoothing cement for repairing the PUR-hot sprayed material subst. No 684.32: EP/PUR-smoothing cement, workable with airless application subst. No 684.33: PUR-sprayed material, workable with airless application or manually Additional notes: object temperature at least 5 °C and at least 3 K above dew point) Table C 4.3.6: Planning resources for materials according to Sheet 84, Annex Area of application Protective system Application Minimum waiting time before subsequent coating at approx. 20 °C System structure Surface preparation Nominal dry film thicknesses [μm] dry wet Vertical and inclined surfaces of - roadway slabs that are in contact with ballast - riveted and welded deck bridges und trough bridges No 684.30/33 ,) Sa 2½ 2000 2000 hot spraying; workable manually or by airless application , ) spray subst. No 684.322), then intersperse quartz sand 0.4 - 0.7 mm subst. No 684.51 2000 2000 process manually or by airless application horizontal surfaces of - roadway slabs that are in contact with ballast - riveted and welded deck bridges and trough bridges subst. No 684.30/33 2,3) Sa 2½ 4000 4000 hot spraying; workable manually or by airless application 4, 5) subst. No 684.322), then intersperse quartz sand 0.4 - 0.7 mm subst. No 684.51 4000 4000 process manually or by airless application tread-resistant walkway surfaces under heavy traffic No 684.32/332) then intersperse quartz sand 0.4 - 0.7 mm subst. No 684.51 Sa 2½ 2000 2000 as above 4) substances as per Sheet 84, Annex are not suitable: − as GB for other TL substances.